electrophoretic deposition of a bioactive si, ca-rich ...· electrophoretic deposition of a...
Post on 20-Aug-2018
Embed Size (px)
Electrophoretic deposition of a bioactive Si, Ca-rich glass coating on 316L stainless steel for biomedical applications H. H. Rodrguez*1, A. Maldonado-Reyes2, D. A. Corts-Hernndez3 1*Universidad Politcnica de Guanajuato Av. Universidad Norte S/N, S/colonia, 38486 Juan Alonso Cortzar, Guanajuato, Mexico 2 Instituto Tecnolgico de Cd. Victoria Apartado Postal 175, 87010 Cd. Victoria, Tamaulipas, Mexico 3 Cinvestav-Unidad Saltillo Carr. Saltillo-Mty, Km 13, Apdo. Postal 663, 25000 Saltillo, Coahuila, Mexico. ABSTRACT This work consisted in the development and characterization of a vitroceramic coating on 316L stainless steel by means of electrophoretic deposition (EPD). This vitroceramic coating was obtained through a Si-, Ca-rich glass coating crystallization. The electrophoretic deposition tests were performed on 316L stainless steel mechanically polished substrates. The results suggest that the electrophoretic coatings adhered well to the metallic surfaces. The results demonstrate that the crystallized coatings are potentially bioactive, because a dense and homogeneous apatite layer, similar to a bone, makes up. Keywords: vitroceramics, electrophoretic deposition, biomaterials, apatite. RESUMEN Este trabajo consisti en el desarrollo y caracterizacin de un recubrimiento vitro-cermico sobre acero inoxidable 316L, obtenido por medio de un proceso de deposicin electrofortica. El recubrimiento vitro-cermico fue obtenido al cristalizar una capa de vidrio rica en calcio y silicio. Las pruebas de deposicin electrofortica fueron realizadas sobre sustratos de acero inoxidable 316L, pulidos mecnicamente. Los resultados sugieren que los recubrimientos electroforticos fueron muy bien adheridos a la superficie metlica. Los resultados demuestran que los recubrimientos cristalizados son potencialmente bio-activos, debido a la formacin de una capa densa y homognea de apatita similar al hueso. 1. Introduction Implants and prostheses, manufactured with bio acceptable metallic materials, do not stick directly to a living bone. On account of this reason, they must be clinically fixed through mechanical interlocking using screws and acrylic cements [1, 2]., Nevertheless, the performance and durability of this type of fixations arethis based on its permanence in the body, its degradation that causes metalosis, and the intensity of the mechanical load that must resist when the patient moves. If the prosthesis fractures or wears offit is given off, it can had been able to cause damage to the adjacent tissue, hemorrhage, pain and the possibility of amputating the=implanted=organ=.
Recently, evidence has been found that plasma- sprayed hydroxyapatite (HA) coatings on metallic substrate formhave evidenced a chemical bond to the bone after its implantation . The intention ofto covering a prosthesis with a material that will form an inter-phase between the bony system and the metallic prosthesis is to obtain an integralable bony chemical fixation, of great durability. OThe osseointegration allows a fixation of the prosthesis to naturally fixateof one natural way. The organism does not attack the metallic prosthesis; this prevents the liberation of with which the metallic ions liberation is prevented. Once the biomaterial is transformed into apatite, the osteogenesis process
remainsstays, ensuringmaking sure a permanent fixation with avoiding no more surgeriesoperations or states pain states for the patient. The moremost widely used technique for the formation of osteointegrables coatings is the fixation by the plasma-sprayed technique. The plasma-sprayed technique is already in clinical use. The covering of hiydroxyapatite by the plasma-sprayed technique, in general, becomes biomimetic apatite after 16 weeks of the implantation. For successful results, the patient must convalesce and be under medical care. Its main disadvantage is the high temperature required in this process, which leads to bioactive layers with defective structures  and which, in addition, damages the substrate of the prosthesis, decrements its mechanical properties as well as its life utility, and compromises the osseointegration. An alternative material for bioactive coatings is wollastonite (W). Wollastonite (TCP/W) glass-ceramics have also shown to be highly bioactive thanks to the formation of apatite on 90% of the surfaces only after 4 weeks of implantation. This is due to the W crystals . A promising technique is electrophoretic deposition (EPD), which offers some interesting advantages such as the feasibility to coat substrates of complex geometries and the ability to form homogenous layers [5, 6]. In addition, this process is simple and inexpensive. The main disadvantage of the EPD technique is the necessity of a subsequent sintering of the coatings, which may damage the metal or alloy mechanical properties. However, this can be used as part of the process to obtain a -TCP/W glass, without coating and substrate structure thermal damage. 2. Materials and methods Metallic substrates were grounded and polished according to the ASTM F-89 standard . The substrates were gently washed, ultrasonically cleaned in ethanol, and stored in desiccators before EPD. In order to obtain a particle smaller than 2 mm, wollastonite (Santa Anita, S. A.) was ball-milled for 5 h, changing direction every 30 minutes.
In order to obtain the glass to be subsequently crystallized in a eutectic material, 19.96 g of SiO2, 58.15 g of CaCO3, and 21.88 g of (NH4)2PO4 were all mixed. Afterwards, this mixture was put in a platinum crucible, and thermally tried at 1450C with a 7C/min rate. When it reached 1450C, it was quickly cooled at room temperature. This material was then dried at 100C for 1 hour, whereupon it was milled in a mortar and agate balls planetary mill. The weight ratio was 4/1 (agate/ceramic). The thus-obtained dust was characterized by MEB and XRD. Spectrophotometric-grade acetone was used as a dispersive medium for EPD . The -TCP/W glass suspension concentration was 4 g/L. The zeta potential was determined by using a Laser Zee Meter (Pem Kem, model 501); a negative value was obtained for the glass/acetone suspension (18.8 mV). This suggests that, in the electrophoretic cell, the working electrode acts as a cathode for the ceramic deposition. The distance between the electrodes was 10 mm. A direct electric current of 800 V was used for 3 min in order to obtain the single glass W/-TCP coating. After its characterization, the coating was crystallized in air at 900 C for 5 h. The heating and cooling rates were 2 C/min. Adhesion measurement was made through a test of tension; a graphic of stress vs. the displacement was obtained. The test was performed following the ASTM F-1501 and F-1044 norms, trial 6.4. The vitroceramic coatings were bonded to a metallic surface with epoxy resin. A simulated body fluid (SBF) with an ionic concentration nearly equal to that of human blood plasma was prepared according to the procedure described by Kokubo et al. . Reagent grade sodium chloride (NaCl), sodium hydrogen carbonate (NaHCO3), potassium chloride (KCl), dipotassium hydrogen phosphate trihydrate (K2HPO43H2O), magnesium chloride hexahydrate (MgCl26H2O), calcium chloride dehydrate (CaCl22H2O), and sodium sulfate (Na2SO4) were all dissolved in deionized water and buffered to pH 7.4 with tris(hydroxymethyl)-aminomethane and 1N HCl at 37 C. The coated substrates were immersed in 250 mL of a SBF at 37 C for 21 days.
The surface of the coatings was characterized by scanning electron microscopy (SEM), energy-dispersive X-ray spectroscopy (EDS), and X-ray diffraction (XRD). The SBF remaining solutions were analyzed with inductively coupled plasma spectrometry (ICP). 3. Results and discussion The change of W/TCP glass deposit weight per surface area, as a function of the applied voltage during EPD, is shown in Figure 1. The homogeneous deposition was obtained at 800V. As observed in Figure 1, the deposit weight increases is increased. The urve of the
figure does not show a decrease concerning the W/TCP glass deposition yield, but the glass color grew dark when the voltage was increased. After the deposition, the coatings were thermally treated at 900C for 5 hours. Figure 2 shows the effect of the temperature on the hardness in the steel 316L. It is observed that to 900C, the hardness is close to 127 HB. The size of the grain before the heat treatment was ASTM 6,479 (Figure 2b), and ASTM 6,11 at the end of the heat treatment (2c). Reason why a significant change in the microstructure of the steel was not observed, so it is deduced that the mechanical properties of this steel, at such temperature, are not decremented.
-20 0 20 40 60 80 100 120 140 160 180 200
Deposition Time (s)
Figure 1. W/TCP glass deposition yield on 316L S.S. as a function of deposition time.
Figure 3a shows the vitroceramic electrophoretical coating microstructure. It shows a homogeneous pore-free surface. After the heat treatment, the microstructure exhibited two phases. With EDX, it was det